9 J Istanbul Univ Fac Dent 2016;50(1):9-18. http://dx.doi.org/10.17096/jiufd.95403
SHEAR BOND STRENGTH OF BRACKETS BONDED TO PORCELAIN SURFACE: IN VITRO STUDY Porselen Yüzeye Yapıştırılan Braketlerin Makaslama Bağlama Kuvveti: İn Vitro Çalışma Fidan Alakuş SABUNCUOĞLU1, Ergül ERTÜRK2 Received: 30/09/2015 Accepted:12/11/2015 ABSTRACT
Purpose: To compare the effects of different porcelain surface treatment methods on the shear bond strength (SBS) and fracture mode of orthodontic brackets. Materials and Methods: Seventy feldspathic porcelain disk samples mounted in acrylic resin blocks were divided into seven groups (n=10) according to type of surface treatment: I, Diamond bur; II, Orthosphoric acid (OPA); III, hydrofluoric acid (HFA); IV, sandblasted with aluminum oxide (SB); V, SB+HFA; VI, Neodymium:yttrium-aluminum-garnet (Nd:YAG) laser; VII, Erbium:yttrium-aluminum-garnet (Er:YAG) laser. Brackets were affixed to treated all-porcelain surfaces with a silane bonding agent and adhesive resin and subjected to SBS testing. Specimens were evaluated according to the adhesive remnant index (ARI), and failure modes were assessed quantitatively under a stereomicroscope and morphologically under a scanning electron microscope (SEM). Statistical analysis was performed using one-way analysis of variance and the post-hoc Tukey test, with the significance level set at 0.05. Results: The highest SBS values were observed for Group V, with no significant difference between Groups V and III. SBS values for Group I were significantly lower than those of all other groups tested. The porcelain/resin interface was the most common site of failure in Group V (40%) and Group III (30%), whereas other groups showed various types of bond failure, with no specific location pre-dominating, but with some of the adhesive left on the porcelain surfaces (ARI scores 2 or 3) in most cases. Conclusion: The current findings indicate that a diamond bur alone is unable to sufficiently etch porcelain surfaces for bracket bonding. Moreover, SB and HFA etching used in combination results in a significantly higher shear-bond strength than HFA or SB alone. Finally, laser etching with either an Nd:YAG or Er:YAG laser was found to be more effective and less time-consuming than both HFA acid and SB for the treatment of deglazed feldspathic porcelain.
Amaç: Farklı porselen yüzey işleme yöntemlerinin, makaslama bağlanma gücü (SBS) ve ortodontik braketlerin kırık modu üzerine olan etkilerini karşılaştırmaktır. Gereç ve Yöntem: Yüzey tedavi tiplerine göre, akrilik bloğa gömülü 70 porselen disk örnekleri 7 gruba (n=10) ayrıldı. I, Elmas frez; II, Ortofosforik asit (OPA); III, hidrofluorik asit (HFA); IV, aluminum oksit ile kumlama (SB); V, SB+HFA; VI, Neodymium:yttriumaluminum-garnet(Nd:YAG) lazer; VII, Erbium:yttrium-aluminumgarnet (Er:YAG) lazer. SBS test uygulamak için, tüm porselen yüzeylere, braketler silan bonding ajan ve adhesive rezin ile tatbik edildi. Örnekler taramalı elektron mikroskop (SEM) ve stereomikroskop altında adezif artık indeks (ARI) ve başarsızlık modlarına göre değerlendirildi. İstatiksel analiz de, anlamlılık seviyesi 0.05 ve tek yönlü varyans analizi ile post-hoc Tukey testi uygulandı. Bulgular: Grup V ve III arasında anlamlı farklılık olmamakla beraber, en yüksek SBS değeri Grup V’de gözlendi. Grup I’in SBS değeri tüm diğer gruplardan daha düşüktür. Porselen/rezin yüzeyinde en fazla başarısızlık Grup V’de (40%) ve Grup III (30%)’dedir. Diğer gruplarda, belli tip olmamakla beraber, çeşitli tip başarısızlıklar porselen yüzeyinde kalan adhesiv de gözlendi (çoğunlukla ARI skor 2 or 3). Sonuç: Braketlerin bondlanması için elmas frezler tek başına yeterli değildir. Fakat SB ve HFA’nın beraber kullanılması HFA ve SB ‘nin tek başına kullanılmasından daha fazla makaslama bağlama kuvveti ile sonuçlanmaktadır. Son olarak, Nd:YAG lazer de, Er:YAG lazer de, deglaze’ li feldspatik porselenlerin tedavisinde, HFA ve SB ‘nin her ikisinden de daha az zaman tüketimine yol açmakta ve daha etkili olmaktadır.
Keywords: Shear bond strength; sandblasting; Er-YAG; Nd:YAG
Anahtar kelimeler: Makaslama bağlanma kuvveti; kumlama; Er-YAG; Nd:YAG
Department of Orthodontics Center for Dental Sciences Maresal Cakmak Hospital Department of Prosthodontics Center for Dental Sciences Maresal Cakmak Hospital
This work is licensed under a Creative Commons Attribution-NonCommercial-NoDerivatives 4.0 International License.
10 Brackets bonded to porcelain Introduction Increases in the number of adults seeking orthodontic treatment has meant that the orthodontist is often faced with the challenge of effectively bonding orthodontic brackets to porcelain restorations (1-3). Because conventional orthodontic bonding systems do not guarantee a level of adhesion to porcelain that is sufficient to withstand orthodontic forces (4), a combination of mechanical and/or chemical conditioning methods is needed to increase the bond strength of orthodontic brackets to porcelain restorations (5). Until now, different surface treatment methods have been used, including sandblasting (SB), hydrofluoric acid application (HFA), orthosphoric acid (OPA) and laser etching. There are several advantages and disadvantages to each of these methods (4, 5). HFA etching has been shown to result in clinically acceptable bond-strength values, but the danger of acid burns must be considered. OPA has been found to be less successful in terms of bond strength than HFA due to an inability to erode superficial layers of silicate porcelain (6-8). Conversely, diamond burs, which may also be used to roughen the porcelain surface, are known to reduce porcelain integrity. Zachrisson et al.(4) have promoted SB, a procedure that involves blasting aluminium-oxide particles onto the porcelain at high pressure to create a microretentive surface, whereas a combination of HFA and SB was found to be a more time-consuming and material-consuming procedure. Laser irradiation has also been mentioned as a promising technique for the surface treatment of porcelain (6, 9) and a number of studies have investigated the effects of Nd:YAG laser etching and Er:YAG laser etching and compared these to other commonly used etching methods. Poosti et al.(9) demonstrated laser irradiation with an Nd:YAG laser to be an acceptable substitute for HFA, whereas an Er:YAG laser was not considered acceptable due to low bond strengths. Similarly, Topcuoglu (10) reported that Er:YAG laser application could not successfully etch porcelain surfaces, and Pich et al.(11) stated that Er:YAG laser cannot be used with dental porcelain because it does not change the chemical composition of dental porcelain surfaces. There is currently no consensus in the literature regarding the best surface conditioning method for producing an optimal bond strength between orthodontic brackets and porcelain restorations, with differences in storage conditions one of the
critical factors in the confusion among study findings. Therefore, the present study was conducted to identify the outcomes of 7 different surface-conditioning methods (diamond bur, orthosphoric acid, hydrofluoric acid, sandblasting, sandblasting+hydrofluoric acid, Nd:YAG laser, Er:YAG laser) in terms of shear-bond strength (SBS) of metal orthodontic brackets to allporcelain (feldspathic) restorative material and bond failure mode. Materials and Methods Specimen Preparation 70 feldspathic porcelain discs (Noritake super porcelain EX-3, Noritake Co., Inc., Nagoya, Japan) with a diameter of 6 mm and a thickness of 3 mm were fabricated and glazed according to the manufacturer’s recommendations (Figure 1). Discs were viewed under a stereomicroscope (EMZTR, Meji Techno Co.,Ltd.,Japan) at 20x magnification to ensure that the flattened surfaces were free from defects such as cracks, pits and fissures. Discs were randomly divided into seven groups (n=10) according to surface conditioning methods, as follows: Group I (DB): Mechanical roughening and deglazing was performed with a cylindrical diamond bur (30 m, Brasseler, Lemgo, Germany) rotated at 40,000 rpm for 3 seconds with the shaft parallel to the sample. Samples were rinsed thoroughly to remove debris and air-dried. Group II (OPA): After roughening and deglazing the porcelain surfaces with a diamond bur as described above, samples were then etched for 2 minutes with 37% orthophosphoric acid (OPA, etching solution, ORMCO, Orange, CA, USA), washed under water for 20 seconds and air-dried. Group III (HFA): After roughening and deglazing the porcelain surfaces with a diamond bur as described above, samples were then etched for 2 minutes with 9.6% hydrofluoric acid gel (HFA, 9.6%, Vita Ceram Etch, Bad Sackingen, Germany) washed under water for 20 seconds and air-dried. Group IV (SB): Samples were sandblasted with a micro-etcher (Micro-Etcher ERC II, Danville Engineering, San Ramon, California, USA) using 50 μm aluminium oxide particles at 60 psi for 3 seconds, with the sandblasting apparatus (Microetcher II, Danville Engineering, San Ramon, California, USA) directed perpendicular to the porcelain surface at a distance of 10 mm. Samples were then washed with water for 20 seconds and air-dried. Group V (SB+HFA): Sandblasting was performed
11 Alakuş Sabuncuoğlu F and Ertürk E. (as described above), followed by HFA etching (as described above). Group VI (Nd:YAG): After roughening and deglazing the porcelain surfaces with a diamond bur as described above, samples were irradiated using an Nd:YAG laser (Figure 2, Fotona, Ljubljana, Slovenia) with a wavelength of 1064nm (300 μm fiber), 2W power and frequency of 10 Hz for 10 seconds in
pulse mode (100μs) using a sweeping motion at approximately 2mm distance from the porcelain surfaces (Figure 3). Group VII (Er.YAG): Samples were treated with laser irradiation as described above for Group VI, but with an Er:YAG laser (2W, 10 Hz, 10 seconds. 2mm (Figure 3).
Figure 1, 2 and 3. From left to right: An example of porcelain disc, the laser system used in the study and laser treatment of porcelain surface. Bonding Procedure Porcelain samples were embedded in acrylic resin blocks, with the smooth surfaces left exposed for bonding. Stainless steel brackets (Rocky Mountain Denver, CO, USA) with approximately the same shape and adhesion area (height: 2mm, base area: 3.5x2.0 mm) as those used for maxillary premolars were used in this study. A silane bonding agent was applied to the exposed porcelain surfaces (Ortho Solo Sealant, Ormco, Orange, CA, USA) and air-thinned, after which an adhesive resin (Enlight Light Cure Adhesive, Ormco, Orange, CA, USA) was prepared and applied to the porcelain surfaces according to the manufacturer’s instructions. Excess resin was
removed with an explorer. Samples were light cured for 40s (Demetron LC, SDS Kerr; light output: 400 mW/cm2), stored in deionized water at 37°C for 24 hours, and thermocycled in water baths at 5°C and 55°C (30-second cycles, total 500 cycles) to simulate temperature and humidity conditions of the oral cavity. Samples were then stored at room temperature in distilled water for 1 week until SBS testing. Shear Bond Strength Testing Shear bond strength was evaluated using a universal testing machine (Shimadzu AG-X, Tokyo, Japan) operating at a speed of 0.5 mm/min. A knifeedged shearing blade was secured on the crosshead with the direction of force parallel to the labial surface
12 Brackets bonded to porcelain and the bracket interface, and the shearing blade struck flush against the edge of the base without touching the porcelain. Values obtained in Newtons (N) were converted into megapascals (MPa) by dividing the value of N by the surface area of the bracket base. After debonding, each sample was examined under a stereomicroscope (Olympus SZ61; Olympus Optical Co, Tokyo, Japan) at 10x magnification to identify the location of bond failure. The residual composite remaining on the premolar was assessed using the Adhesive Remnant Index (ARI), which scores each sample according to the amount of material remaining on the porcelain surface, as follows: 0, no adhesive remaining; 1, less than 50% of the adhesive remaining; 2, more than 50% of the adhesive remaining; 3, all of the adhesive remaining on the porcelain surface, with a distinct impression of the bracket base.
Statistical Analysis Statistical analysis was performed using the Statistical Package for Social Sciences, Windows v. 10.0.0 (SPSS Inc., Chicago, Illinois, USA). Descriptive statistics including means, standard deviations and minimum and maximum values were calculated for each group. A Kolmogorov-Smirnov normality test was applied and showed normality of distribution; thus, one-way analysis of variance (ANOVA) and post-hoc Tukey tests were used to identify differences in SBS among groups with the level of significance set at p